Introduction to Unconventional Superconductivity Manfred Sigrist
Total Page：16
File Type：pdf, Size：1020Kb
Introduction to Unconventional Superconductivity Manfred Sigrist Theoretische Physik, ETH-Hönggerberg, 8093 Zürich, Switzerland Abstract. This lecture gives a basic introduction into some aspects of the unconventionalsupercon- ductivity. First we analyze the conditions to realized unconventional superconductivity in strongly correlated electron systems. Then an introduction of the generalized BCS theory is given and sev- eral key properties of unconventional pairing states are discussed. The phenomenological treatment based on the Ginzburg-Landau formulations provides a view on unconventional superconductivity based on the conceptof symmetry breaking.Finally some aspects of two examples will be discussed: high-temperature superconductivity and spin-triplet superconductivity in Sr2RuO4. Keywords: Unconventional superconductivity, high-temperature superconductivity, Sr2RuO4 INTRODUCTION Superconductivity remains to be one of the most fascinating and intriguing phases of matter even nearly hundred years after its ﬁrst observation. Owing to the breakthrough in 1957 by Bardeen, Cooper and Schrieffer we understand superconductivity as a conden- sate of electron pairs, so-called Cooper pairs, which form due to an attractive interaction among electrons. In the superconducting materials known until the mid-seventies this interaction is mediated by electron-phonon coupling which gises rise to Cooper pairs in the most symmetric form, i.e. vanishing relative orbital angular momentum and spin sin- glet conﬁguration (nowadays called s-wave pairing). After the introduction of the BCS concept, also studies of alternative pairing forms started. Early on Anderson and Morel [1] as well as Balian and Werthamer [2] investigated superconducting phases which later would be identiﬁed as the A- and the B-phase of superﬂuid 3He [3]. In contrast to the s-wave superconductors the A- and B-phase are characterized by Cooper pairs with an- gular momentum 1 and spin-triplet conﬁguration. This was the beginning of the era of unconventional superconductivity, condensates of Cooper pairs of lower symmetry, in contrast to the conventional superconductors with the most symmetric Cooper pairs. The discovery of superﬂuidity in the 3He in 1971 by Osheroff, Richardson and Lee gave the ﬁrst example of unconventional Cooper pairing [4]. In 3He other pairing mecha- nisms are obviously of non-phononic origin, based on van der Waals and spin ﬂuctuation mediated interactions [3, 5]. Moreover, 3He is the prime example for a strongly corre- lated Fermi liquid where the short range repulsive interaction leads to strong renormal- isations of the quasiparticle mass and other quantities. Alternative pairing mechanism and strong correlation effects are key elements to prevent electrons from undergoing conventional s-wave pairing. The natural aim to ﬁnd among solids a system with unconventional Cooper pairing was not satisﬁed until much latter when at the end of seventies and beginning of the eighties two novel classes of strongly correlated materials were found among which some were superconducting - the heavy Fermion compounds [6, 7, 8] and organic con- ductors [9, 10]. The ﬁrst type of materials are intermetallics containing rare earth ions and the second are highly anisotropic conductors based organic units. Although it is not clear until today which form of Cooper pairing is realized in many of these materials, some of them possess complex phase diagrams with several different superconducting phases, ﬁrmly establishing the unconventional nature. In both types of material super- conductivity emerges out of phase that are nearly magnetic or evolve under pressure from a magnetically ordered state. In 1986 the discovery of high-temperature supercon- ductivity in cuprate compounds with layered perovskite structure announced the era of unconventional superconductivity to a wider community [11]. This system dominates to the present days the study of superconductivity. A few years were necessary to estab- lish the unconventional character to pairing for the cuprates. Cooper pairs possess in the quasi-two-dimensional systems a so-called spin singlet dx2 y2-wave structure [12, 13]. In cuprate materials the important role of magnetism in the c−ontext of the unusual metal- lic properties and superconductivity is underlined by the fact that this superconductor emerges from an antiferromagnetic Mott-insulator upon carrier doping [14]. The essential role which magnetism could play for unconventional superconductivity became one of the guiding strategies in the nineties in the search for new materials. Striking examples of superconductivity associated with magnetic phases are several Ce- based compounds where superconductivity is associated with a quantum critical point of an antiferromagnetically ordered phase. CeIn3 [15], CePd2Si2 [15, 16] and CeMIn5 (M=Co,Rh,Ir) [17, 18] are a few examples of this type. Surprisingly superconductivity was also found inside a ferromagnetic phases in UGe2 [19], URhGe [20] and ZrZn2 [21], possibly connected with the corresponding magnetic quantum phase transition. Sr2RuO4 whose superconductivity was discovered in 1994 deserves a special place as an exemplary case of an unconventional superconductor resulting from a strongly correlated Fermi liquid phase [22]. In various respects it may be considered as an analog to 3He, including the pairing symmetry which is closely related to the A-phase of the superﬂuid. Many aspects of this superconductor have been explored in much detail during the last ten years [23, 24] More recently the superconducting skutterudites such as PrOs4Sb12 have been aroused much interest as new examples of heavy Fermion materials with multiple superconducting phases [25]. The exploration of superconductivity in materials with geometrically frustrated crystall lattices has been a further recent focus. This in- cludes NaxCoO4 intercalated with water which has been considered as a realization of superconductivity on a triangular lattice [26]. Also superconductivity in metalls with the pyrochlor structure belong to this class such as Cd2Re2O7 [27] and AOs2O6 (A=Cs,Rb,K) [28], although it is not clear whether they are unconventional. Crystal structure can have an even crucial impact on superconductivity than in the case of frustrated lattices, if inversion symmetry is missing. As we will see later inversion together with time reversal invariance are among the key symmetries for Cooper pair formation. The discovery of superconductivity in the heavy Fermion systems CePt3Si and UIr have reopened the discussion of superconductivity in this kind of systems [29]. During the past two decades we experience important developments in the ﬁeld of unconventional superconductivity, from the side of new materials as well as theoretical understanding. New strategies for the discovery of unconventional superconductors bear fruits besides the tremendous progress in sample production which is a mandatory accessory for the observation of unconventional superconducting phases which are very sensitive to material disorder effects. These lecture notes cover a few aspects and developments in the ﬁeld of unconventional superconductivity. Naturally this overview is selective and the viewpoint is biased by the preferences of the lecturer. CONVENTIONAL VERSUS UNCONVENTIONAL SUPERCONDUCTIVITY The most fundamental experimental aspect of superconductivity is the screening of a magnetic ﬁeld, the Meissner-Ochsenfeld effect, which implies also the existence of per- sistent electric currents. The microscopic theory which provides such a feature is based on the coherent state introduced by Bardeen, Cooper and Schrieffer. In this chapter we will give a brief introduction to this BCS state (screening effects, however, will be only addressed later in the context of the phenomenological Ginzburg-Landau formulation) and motivate the generalization beyond the standard BCS theory of conventional super- conductivity. We will compare also the electron-phonon mechanism for superconduc- tivity with possible alternative mechanisms, in particular, based on effective interaction originating from spin ﬂuctuations. Standard BCS theory It is convenient for the further discussion to ﬁrst introduce the basics of the meanﬁeld formulation of the BCS theory using a very simple model. The formation of Cooper pairs which is at the heart of the microscopic theory of Bardeen, Cooper and Schrieffer, requires the presence of an attractive interaction between electrons. For our purpose it is sufﬁcient to use a structureless contact interaction which yields the following Hamiltonian in a second-quantization language, ξ † † † H = ∑ ~ c c~ + g ∑ c c c~ c~ . (1) k ~k s k s ~k +~q, ~k ~q, k 0 k ~ ~ ~ ↑ 0− ↓ ↓ ↑ k ,s k ,k 0,~q where c† (c ) creates (annihilates) an electron with momentum ~k and spin s. The ~k s ~k s ﬁrst term is the kinetic energy accounting for the band structure of the metal, where ξ µ ξ ε µ h¯ 2 ~ 2 2 ~k is measured relative to the chemical potential , i.e. ~k = ~k = 2m (k kF ) for a parabolic band. The second term describes the two-particle− interaction which− is represented by a structureless scattering matrix element g. This corresponds to a ~ δ ~ attractive contact interaction U(~r r0 ) = g (~r r0 ) (with g < 0) such that V~ ~ = − − k ,k 0 3 i~q ~r V(~q = ~k ~k 0) = d rU(~r)e · = g. Note that in this case only particle of opposite spin interact.− R For the BCS theory the relevant scattering processes are those of particle pairs with vanishing total momentum, belonging to the set